- Open Access
Adhesive joint computations using cohesive zones
© Valoroso and de Barros; licensee Springer. 2013
- Received: 4 October 2013
- Accepted: 3 December 2013
- Published: 30 December 2013
The cohesive zone approach has gained increasing success in recent years for simulating debonding and fracture via finite element methods and is ideally suited for simulating adhesive joints, the potential crack paths being generally known in advance in most cases. In the paper the determination of the size of the so-called cohesive process zone is discussed, i.e. the region wherein the stress and damage state have to be correctly resolved in order to properly quantify the dissipated energy and the load bearing capacity of the structure. An a priori estimate for the size of the active process zone is provided based on the beam on elastic foundation model in which the material parameters of the cohesive law are incorporated.
The formulation of the cohesive model in a damage mechanics format is first provided. The beam on elastic foundation model is then recalled and an approximate solution for the cohesive zone length is found that depends on a material length and a geometric parameter as well.
Results and discussion
Numerical results are presented for a Double Cantilever Beam (DCB) geometry with varying thickness for which bilinear and exponential cohesive laws are considered. The influence of the geometry and of the shape of the cohesive law are put forward in terms of global response and evolution of the cohesive process zone.
The size of the process zone is found to be quite sensitive to the specimen characteristic size, whose influence is well captured even using a simplified modeling wherein the original cohesive law is changed into an ideal perfectly brittle one. This leads to fairly good estimates of the size of the cohesive zone compared to finite element results.
- Adhesive joints
- Cohesive zone
- Interface elements
Recent advances in adhesive bonding technologies have led to a rapid growth in the use of structural adhesives and in many cases their use is by far more convenient than traditional joining methods [1, 2]. Namely, a major advantage of structural adhesive joints is that they provide more uniform stress transfer compared to other types of fastening systems; however, most adhesive bonds contain defects such as voids, regions with no or poor bonding and micro cracks, and such defects might grow under loading and give rise to local decohesion and formation of macro fractures.
To a great extent, at the onset of decohesion in a bonded joint the surface tractions between the joined adherends do not suddenly drop to zero owing to the presence of low-range interactions that precede the formation of traction-free surfaces. Such interactions can be effectively described by allowing jumps in the displacement field along an interface where crack propagation is known or is expected to occur. At each point of the interface such displacement discontinuities have then to be related to surface tractions components via a decohesion model, i.e. a relationship able of representing the different phases of the potential debonding process from the initial undamaged condition to progressive damage and up to fracture propagation. The driving idea for such a class of models is the cohesive-zone concept initially introduced by Barenblatt  and Dugdale . This approach has gained major popularity in recent years for simulating delamination, debonding, fracture and fragmentation via finite element methods and is ideally suited for simulating adhesive joints, the potential crack paths being generally known in advance in most cases, see e.g. [5, 6] and references therein for recent survey accounts.
Adhesive joints may be loaded to failure in the design configurations or in the form of test specimens and it is important to fully understand the response obtained by such testing especially for the apparently simple configurations used in international standards since fracture behavior is in general governed by material properties, loading conditions and geometrical parameters as well. Moreover, apart from being employed for studying sensitivity and data reduction [7, 8], simple joint configurations can be interpreted on a theoretical basis to define requirements for elements and for the mesh that guarantee meaningful answers from numerics. This is indeed a crucial point since it has a direct impact on the results of computations.
In this paper one of such critical aspects of finite element analysis of adhesive joints is discussed, i.e. the estimation of the size of the cohesive process zone. This is the region wherein the stress and damage state must be correctly resolved to properly quantify the dissipated energy and the load bearing capacity of the structure.
It is well known that a cohesive model brings a length scale into the problem in the form of a characteristic length parameter; this expresses the length over which the cohesive constitutive relation plays a role. A recent survey about length scales in the simulation of delamination and fracture can be found in ; worth mentioning is also Reference , where is provided a table comparing the different expressions proposed in the literature to estimate the cohesive zone extension.
Based on a simplified modeling, in the present work an a priori estimate for the size of the active process zone under mode-I conditions, and for the size of the nearby region subject to compressive stresses as well, is provided. To this end use is made of a beam on elastic foundation model in which the material parameters of the cohesive law are incorporated. The expressions obtained that quantify the extension of the cohesive zone are fairly accurate and very easy to implement. This is demonstrated through numerical experiments in which we consider two different shapes of the traction-separation law and simulate two symmetric double cantilever beam (DCB) fracture specimens with different characteristic geometric size.
In the above relationships t and Y respectively denote the interface traction and the damage-driving force, D ∈ [0, 1] is the scalar damage variable, [[u]] is the displacement jump in the direction normal to the interface, 〈·〉± indicates the positive (negative) parts of the argument while k and k- are the undamaged interface stiffness parameters in tension and compression, respectively.
Beam on elastic foundation model
The idea of using the beam on elastic foundation model to analyze adhesively bonded specimens is not new. In earlier applications it has been employed in the form of the one-parameter Winkler model to compute corrections factors for the DCB specimen for data reduction based on beam theories , see also .
In closing this section we remind that, apart from the factor (2/3)1/4≃0.9, the expression (12) is usually taken to represent the length of the cohesive damage zone in slender composite laminates .
The cohesive model summarized in the previous Section has been implemented in a customized version of the finite element code FEAP . For the computations described in this section use has been made of enhanced assumed strain quadrilaterals for the bulk material and 4-noded interface elements.
As a numerical example we refer to the classical DCB geometry under plane strain conditions. Loading is simulated via displacement control and either a bilinear or an exponential cohesive law are considered. For results to be comparable the same critical fracture energy G c = 0.125 N/mm and peak stress t max = 10 N/mm2 have been taken as material parameters for the interface, which are representative of a thin epoxy adhesive film (≃ 0.2 mm thick) bonded on an aluminum substrate. Elastic moduli for the bulk material (aluminum alloy) are E = 70 GPa and ν = 0.3. The specimen length is L = 200 mm, the initial flaw is a = 50 mm and the arm height is taken as h = 8 mm for the thin beam and h = 80 mm for the thick case. Unlike the thin beam, which corresponds to the geometry that has been experimentally tested in , the thick beam case is a pure numerical exercise aiming to reproduce a stiff structure for which the size of the cohesive zone is comparable to the dimensions of the sample, see also .
From the beam on elastic foundation model the size of the cohesive zone follows from relationship (10) for n = 0, i.e. as the first zero of the deflection function (5), whereby one obtains a length x0 = 11.8 mm when using the stiffness-preserving wavelength (6) and x0 = 6.31 mm when expression (12) is adopted instead. The interval defined by these values clearly delimits the length of the damage cohesive zone computed via finite elements whereas the material length parameter defined in (7) is computed as l c = 87.5 mm, which is quite far from the numerical solution. As for the size of the region subject to compressive stresses ahead of the crack front, from finite element computations one obtains a length of about 30 mm while from (10) one obtains x1 - x0 = π / λ ∈[25.6, 41.3] mm, which again includes the numerically computed value.
For the case at hand of the thick specimen, no steady state is reached in the evolution of the cohesive zone size that starts decreasing right after the peak load has been attained. The maximum length for the damage cohesive zone computed via finite element analysis is found to be lcoh,exp = 63.5 mm for the exponential cohesive law and lcoh,bil = 39.2 mm for the bilinear one whereas from the Winkler model the size of the cohesive zone is estimated either as x0 = 44.5 mm if the wavelength is computed using (6) or as x0 = 87.8 mm when referring to (12). Obviously, the length parameter (7) is the same as before since, by definition, it is independent from the specimen size. As for the size of the region subject to compressive stresses ahead of the crack front, it is numerically found to extend up to the right free end of the specimen. This is confirmed from (10) as well, whereby it is estimated as x1 - x0 = π / λ ∈[130.6, 232.2] mm, which practically exceeds the specimen length.
Based on the previous results one could conclude that the size of the cohesive process zone is captured fairly well for both the thin and thick DCB cases, which demonstrates the importance of using an estimate that includes a geometric parameter in addition to the material length scale (7). Despite the intrinsic limitations of the adopted simplified modeling, that basically relies upon linear elastic considerations, the a priori estimates for the size of both the cohesive zone and of the compressed region ahead of the crack front seem to be reliable especially for the thin DCB case. On the contrary, for the thick DCB a priori estimates do not compare well as in the previous case; this is likely to occur because for the thick DCB the cohesive zone is not completely developed since the beam cannot be considered long compared to the model wavelength.
A simplified modeling for estimating the cohesive zone size in mode-I debonding problems across a range of geometrical properties has been presented. In particular, it is shown that the size of the damaged zone and that of the region subject to compressive stresses ahead of the crack front can be estimated with good approximation as functions of the cohesive parameters and of the specimen geometry via a beam on elastic foundation model. Unlike the global load-deflection response, for a given characteristic length of the traction-separation law the size of the process zone is found to be quite sensitive to the specimen characteristic size, whose influence is well captured even using a simplified modeling.
In the present paper comparisons between finite element results and the beam model have been carried out by modifying the shape of the cohesive law in a way to preserve either the initial stiffness or the peak stress. This has led to fairly good estimates of the size of the cohesive zone. In the Authors’ opinion the subject is worth investigating and alternative strategies to improve the predictive capabilities of the present approach will be examined in forthcoming papers.
- Adams RD: Adhesive Bonding: Science, Technology and Applications. Boca Raton: CRC Press; 2005.View ArticleGoogle Scholar
- da Silva LFM, Ochsner A, Adams RD (Eds): Handbook of adhesion technology. Heidelberg: Springer; 2011.Google Scholar
- Barenblatt GI: The Mathematical Theory of Equilibrium Cracks in Brittle Fracture. In Advances in Applied Mechanics, vol 7.. Edited by: Dryden HL, von Kármán Th, Kuerti G, van den Dungen FH, Howarth L. Elsevier; 1962:55–129. http://dx.doi.org/10.1016/S0065–2156(08)70121–2Google Scholar
- Dugdale DS: Yielding of steel sheets containing slits. J Mech Phys Solids 1960, 8(2):100–104. 10.1016/0022-5096(60)90013-2View ArticleGoogle Scholar
- Valoroso N, Sessa S, Lepore M, Cricrì G: Identification of mode-I cohesive parameters for bonded interfaces based on DCB test. Eng Fracture Mech 2013, 104(1):56–79.View ArticleGoogle Scholar
- Campilho RDSG, Banea MD, Neto JABP, da Silva LFM: Modelling adhesive joints with cohesive zone models: effect of the cohesive law shape of the adhesive layer. Int J Adhesion Adhesives 2013, 44: 48–56.View ArticleGoogle Scholar
- Valoroso N, Fedele R: Characterization of a cohesive-zone model describing damage and de-cohesion at bonded interfaces: sensitivity analysis and mode-I parameter identification. Int J Solids Struct 2010, 47(13):1666–1677. 10.1016/j.ijsolstr.2010.03.001View ArticleGoogle Scholar
- Fedele R, Sessa S, Valoroso N: Image correlation-based identification of fracture parameters for structural adhesives. Technische Mech 2012, 32(2):195–204.Google Scholar
- Harper PW, Hallett SR: Cohesive zone length in numerical simulations of composite delamination. Eng Fracture Mech 2008, 75(16):4774–4792. 10.1016/j.engfracmech.2008.06.004View ArticleGoogle Scholar
- Turon A, Dávila CG, Camanho PP, Costa J: An engineering solution for mesh size effects in the simulation of delamination using cohesive zone models. Eng Fracture Mech 2007, 74(10):1665–1682. 10.1016/j.engfracmech.2006.08.025View ArticleGoogle Scholar
- Valoroso N, Champaney L: A damage-mechanics-based approach for modelling decohesion in adhesively bonded assemblies. Eng Fracture Mech 2006, 73(18):2774–2801. 10.1016/j.engfracmech.2006.04.029View ArticleGoogle Scholar
- Williams JG: End corrections for orthotropic DCB specimens. Composites Sci Technol 1989, 35(4):367–376. 10.1016/0266-3538(89)90058-4View ArticleGoogle Scholar
- Williams JG, Hadavinia H: Analytical solutions of cohesive zone models. J Mech Phys Solids 2002, 50(4):809–825. 10.1016/S0022-5096(01)00095-3View ArticleGoogle Scholar
- Timoshenko SP, Goodier JN: Theory of elasticity,. Singapore: McGraw Hill; 1970.Google Scholar
- Hillerborg A, Modéer M, Petersson P-E: Analysis of crack formation and crack growth in concrete by means of fracture mechanics and finite elements. Cement Concrete Res 1976, 6(6):773–781. 10.1016/0008-8846(76)90007-7View ArticleGoogle Scholar
- Yang Q, Cox B: Cohesive models for damage evolution in laminated composites. Int J Fracture 2005, 133(2):107–137. 10.1007/s10704-005-4729-6View ArticleGoogle Scholar
- Taylor RL: FEAP - Programmer Manual. 2013.http://www.ce.berkeley.edu/projects/feap/pmanual84.pdfGoogle Scholar
- Alfano G, de Barros S, Champaney L, Valoroso N: Comparison between two cohesive-zone models for the analysis of interface debonding. In European Congress on Computational Methods in Applied Sciences and Engineering. Edited by: Neittaanmäki P, Rossi T, Majava K, Pironneau O. Finland: University of Jyväskylä, Department of Mathematical Information Technology; 2004.Google Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License(http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.